Guest Tunable Structure and Spin Crossover Properties in a Nanoporous Coordination Framework Material
Suzanne M. Neville; Gregory J. Halder; Karena W. Chapman; Martin B. Duriska; Boujemaa Moubaraki; Keith S. Murray; Cameron J. Kepert; Journal of the American Chemical Society 131 (2009) 12106–12108; doi:10.1021/ja905360g

data_4104953
_publ_contact_author_address
; 
School of Chemistry
University of Sydney
NSW 2006
Australia
;
_publ_contact_author_email       c.kepert@chem.usyd.edu.au
_publ_contact_author_fax         +61-2-9351-3329
_publ_contact_author_name        'Prof. Cameron J. Kepert'
_publ_contact_author_phone       +61-2-9351-5741
_publ_section_title
;
 Guest Tunable Structure and Spin Crossover Properties in a Nanoporous
 Coordination Framework Material
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              12106
_journal_page_last               12108
_journal_paper_doi               10.1021/ja905360g
_journal_volume                  131
_journal_year                    2009
_chemical_formula_moiety         'C30 H32 Fe N6 O4 S2, 3(C O)'
_chemical_formula_sum            'C33 H32 Fe N6 O7 S2'
_chemical_formula_weight         744.62
_chemical_name_common            SCOF-2(Me)as
_space_group_IT_number           130
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-P 4a 2ac'
_symmetry_space_group_name_H-M   'P 4/n c c :2'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   14.675(3)
_cell_length_b                   14.675(3)
_cell_length_c                   17.984(7)
_cell_measurement_reflns_used    111
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      18.0111
_cell_measurement_theta_min      2.7232
_cell_volume                     3873.0(19)
_computing_cell_refinement       'SMART (BrukerAXS, 1997)'
_computing_data_collection       'SMART (BrukerAXS, 1997)'
_computing_data_reduction        'SAINT+ (BrukerAXS, 1997)'
_computing_molecular_graphics    'MERCURY 1.4 (Bruno et al., 2002)'
_computing_publication_material  'XCIF V6.12 (BrukerAXS, 2001).'
_computing_structure_refinement  X-SEED
_computing_structure_solution    'SHELXS86 (Sheldrick, 1990)'
_diffrn_ambient_temperature      200(2)
_diffrn_measured_fraction_theta_full 0.985
_diffrn_measured_fraction_theta_max 0.985
_diffrn_measurement_device_type  'Bruker SMART 1000'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0684
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            2315
_diffrn_reflns_theta_full        27.99
_diffrn_reflns_theta_max         27.99
_diffrn_reflns_theta_min         2.26
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.547
_exptl_absorpt_correction_T_max  0.8891
_exptl_absorpt_correction_T_min  0.8663
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   sadabs
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.277
_exptl_crystal_description       rod
_exptl_crystal_F_000             1544
_exptl_crystal_size_max          0.27
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.22
_refine_diff_density_max         0.618
_refine_diff_density_min         -1.119
_refine_diff_density_rms         0.124
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.110
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     118
_refine_ls_number_reflns         2315
_refine_ls_number_restraints     10
_refine_ls_restrained_S_all      1.109
_refine_ls_R_factor_all          0.1852
_refine_ls_R_factor_gt           0.0790
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1101P)^2^+26.2893P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1910
_refine_ls_wR_factor_ref         0.3054
_reflns_number_gt                1113
_reflns_number_total             2315
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja905360g_si_001_4.cif
_cod_data_source_block           SCOF-2(Me)as
_cod_original_cell_volume        3873.1(18)
_cod_original_sg_symbol_H-M      'P 4/n c c'
_cod_database_code               4104953